science china chemistry - national chiao tung university ?· science china chemistry ... because...
Post on 09-Apr-2019
Embed Size (px)
SCIENCE CHINA Chemistry
Science China Press and Springer-Verlag Berlin Heidelberg 2010 chem.scichina.com www.springerlink.com
*Corresponding author (email: firstname.lastname@example.org; email@example.com; firstname.lastname@example.org)
REVIEWS August 2010 Vol.53 No.8: 16791694 doi: 10.1007/s11426-010-4043-7
Molecular hosts for triplet emitters in organic light-emitting diodes and the corresponding working principle
MI BaoXiu1,2, GAO ZhiQiang1*, LIAO ZhangJin2, HUANG Wei2* & CHEN Chin Hsin3*
1Jiangsu Engineering Center for Flat-Panel Displays & Solid-State Lighting; School of Materials Science & Engineering, Nanjing University of Posts & Telecommunications, Nanjing 210046, China
2Key Laboratory for Organic Electronics & Information Displays (KLOEID), Institute of Advanced Materials (IAM), Nanjing University of Posts & Telecommunications, Nanjing 210046, China
3Display Institute, Microelectronics and Information Systems Research Center, National Chiao Tung University Hsinchu, Hsinchu, 300 China
Received March 24, 2010; accepted April 24, 2010
This paper summarizes the mechanism and routes for excitation of triplet emitters in dopant emission based phosphorescent organic light-emitting diodes (PhOLEDs), providing a comprehensive overview of recent progress in molecular hosts for trip-let emitters in PhOLEDs. Particularly, based on the nature of different hosts, e.g., hole transporting, electron transporting or bipolar materials, in which the dopant emitters can be hosted to generate phosphorescence, the respective device performances are summarized and compared. Highlights are given to the relationships among the molecular structure, thermal stability, trip-let energy, carrier mobility, molecular orbital energy level and their corresponding device performances.
phosphorescent organic light-emitting diodes (OLEDs), working principle, electrophosphorescence, hosts, triplet emitter
Organic light-emitting diodes (OLEDs) are current driven emissive-devices in which organic materials are used as active elements. Compared to their inorganic counterpart, organic materials have the advantages of low-cost synthesis, functional tunability, flexibility and good thin film-forming ability. The devices based on organic materials are generally capable of simple and low-temperature manufacture processes such as spin-coating, ink-printing, and dipping, hence less expensive. Organic materials bear the potentials for large- area fabrication, flexible substrates, and are environmentally friendly. In the past two decades, OLEDs have been intensively studied, due to their potential application for next generation flat panel displays (FPDs) and solid state lighting (SSL).
OLEDs utilizing phosphorescent materials as emitters (PhOLEDs) are more attractive than those based on fluo-rescent emitters because of their ability to harvest both singlet and triplet excitons, hence reaching 100% internal quantum efficiency [1, 2]. Non-doped PhOLEDs for blue , green [4, 5], orange , and red [7, 8] were demon-strated. However, those devices usually face the problem of luminescence quenching from the condensed state of emit-ters. In addition, it is not an economical consideration to apply phosphorescent materials as hosts, because the phos-phors which generally consist of transition metals of Ir or Pt are very expensive due to the high cost of starting materials and synthesis. Moreover, doped OLEDs have been demon-strated to possess prolonged operational lifetime without significant concentration quenching [9, 10]. In doped OLEDs, the carrier injection barrier between the emitting layer (EML) and adjacent carrier transport layers as well as the carrier transporting ability of EML can be adjusted fea-sibly by the host, adding flexibility for the design of device
1680 MI BaoXiu, et al. Sci China Chem August (2010) Vol.53 No.8
structures. This can also simplify the molecular design, be-cause the electronic and photo-physical requirements of EMLs can be considered separately with the former prop-erty mainly depending on the host and the latter dominated by the dopant. Thus, most work in the field of PhOLEDs focused on phosphorescent guest-host system.
To disclose the device mechanisms and realize the PhOLED application, a huge number of research works, including many good review articles , were pub-lished. However, despite the fact that the investigation of suitable host materials for triplet emitters has been con-ducted extensively since the early stage of PhOLEDs re-search , there are rare reviews focusing on this aspect. Here, the mechanism and scenarios for energy transfer from the host to the triplet dopant are summarized and discussed, and the molecular host materials for phosphorescent dopant emitters are reviewed. In particular for host materials, after the discussion of basic characterization methods for the host materials, recent advances directed towards the molecule design as well as their application in devices are addressed. The phosphorescent dopant materials that are discussed in the following parts are shown in Figure 1. We used iridium complexes as representative dopants, because these materi-als show the best performance among phosphorescent mate-rials, and are the utmost promising ones for applications.
Figure 1 Molecular structures of phosphorescent dopants discussed in this work. The numbers in unit of nm indicate their emission peaks in dis-persion (either film or solution).
2 Excitation of triplet emitters dispersed in the host under an electric field
Figure 2(a) shows the basic device architecture for dopant emitter based PhOLEDs, including the hole transport layer (HTL), doped emitting layer (EML) and electron transport layer (ETL) in sequence, sandwiched between two elec-trodes. Attributed to the long lifetime of the phosphorescent emitter, PhOLEDs usually suffer from large efficiency roll- off at high current density , which can be relieved by the selection of the phosphorescent materials with short triplet lifetime, the suitable host material, and the judicious design of device structure such as insertion of the carrier/ exciton block layer or buffer layer . Among them, the design of suitable host materials for PhOLEDs is a challenging task, because complex and competing channels exist for host/dopant emitters to be excited as well as for excitons to be confined in the EML, as shown in Figure 2(b). Generally, the ways of electrical excitation of the dopant emitter in PhOLEDs can be categorized into two types: one is direct recombination of carriers on dopants (charge trap) and the other is energy transfer from the excited host.
The favorable charge trap requires the HOMO/LUMO level of the dopant locate above/below that of the host, re-spectively. In this case, the dopant is likely to act as a hole/electron trap. Sequentially, the trapped holes/electrons on the dopant may provide sites for electron-hole recombi-nation, forming a variety of excited states, such as singlet and triplet excitons. In phosphorescent emitters, it is gener-ally believed that the intersystem crossing (ISC) process from the singlet to the triplet occurs with high probability, thus singlet excitons are expected to transfer to the corre-sponding triplet state efficiently. Due to the strong spin or-bital coupling, strong phosphorescence can be produced via the dominant radiation decay process of triplet excitons. Figure 2(b) illustrates these reaction channels.
Energy transfer is the most significant process in dopant emitter based OLEDs and mainly includes Frster energy transfer and Dexter energy transfer (in Figure 2(b), repre-sented as thin arrow lines and broad arrow lines, respec-tively). The criteria for efficient Frster energy transfer are (1) good spectra overlap between the emission of the host and the absorption of the dopant, (2) strong to moderate emission of the host, (3) strong absorption of the dopant, and (4) within 100 separation between host and dopant molecules. Good Dexter energy transfer must meet (1) spectra overlap between the emission of the host and the absorption of the dopant to provide orbital overlap of the two concerned energy levels, (2) spin conservation, and (3) within 10 separation between host and dopant molecules to render spatial vicinity.
Accordingly, in the viewpoint of energy transfer from the host to the triplet state of the dopant, possible mechanisms can be described as follows (refer to Figure 2(b)):
MI BaoXiu, et al. Sci China Chem August (2010) Vol.53 No.8 1681
Figure 2 (a) Layered OLEDs structure with a dopant emitter. (b) The main ways for the triplet dopant to be excited under an electric field.
H D H D H D1 0 0 1 0 1
H D H D H D1 0 0 1 0 1
H D H D H D1 0 0 1 0 1
H D H D1 0 0 1
(I) : S S S S S T
(II) : S S S S S T
(III) : T S S S S T
(IV) : T S S T
F rster ISC
F rster ISC
where singlet and triplet states are represented by S and T, respectively; the subscript 1 and 0 indicate an excited state and the ground state, respectively; the superscript H and D refer to the host and the dopant, respectively; ISC means inter-system crossing; Frster and Dexter refer to Frster and Dexter energy transfer, respectively. (I) and (II) are the main routes for energy transfer from the singlet excited state of the host to the triplet of the dopant, while (III) and (IV) represent the dominant channels of those from the triplet excited state of the host to the triplet of the dopant.
It is noteworthy that energy transfer from the singlet of the host (S